PHYSICAL REVIEW B

VOLUME 36, NUMBER 3

15 JULY 1987-II

Metallic surfaces in the Thomas —Fermi —von Wei*sacker approach: Self-consistent solution Constantino

A. Utreras-Diaz

(Received 17 November

1986)

The problem of a metallic surface is studied and solved in the Thomas —Fermi —von Weizsacker approach. The analysis of the asymptotic solutions shows that the electronic density n (x) approaches its bulk value no in the metal interior exponentially, oscillating about it. This behavior is found to be an effect of the von Weizsacker term, rather than of the exchange-correlation interaction, as one may have thought. The Euler equation is solved for a slab geometry, calculating work functions and surface energies of several simple metals. The case of the pseudojellium model, recently introduced, is also considered here. The results are compared with those of the exact Lang-Kohn theory and with those of Smith.

INTRODUCTION

the local-density

The problem of a metallic surface has been studied using a variety of approaches over the years. The progress that we have witnessed in recent years has been made theory' (DFT). largely possible by the density-functional In considering a given problem within the DFT, one can choose to solve the Kohn-Sham equations for the system, an approach that was pioneered by Lang and Kohn for metallic surfaces. The other approach available consists in solving the Euler equation for the electronic density. In the last case one needs to have accurate expressions for the kinetic-energy functional. An alternative method has been to use the variational principle; for the problem of metallic surfaces this was first done by Smith, who minimized the energy with respect to variations of the electronic density within a one-parameter family of functions. The Euler equation was solved by Warner for a cesium slab. However, his discussion of this subject was incomplete, and has remained unnoticed by most workers in the field. This work is organized as follows. In Sec. I the mathematical problem is set up, and some exact results concerning the nature of the asymptotic solutions are discussed. Section II is devoted to the discussion of the numerical approach, boundary conditions, and stability. Numerical results are presented and discussed in Sec. III.

I.

f

The .

(1)

Here n (x) is the electronic density and n+(x) denotes the density of the ionic background. The kinetic-energy functional is taken as the Thomas-Fermi term plus the first gradient correction (the von Weizsacker term),

A,

= '. —,

f

[3(3m. n)

i 10+A(dn/ndx) /8]n

The exchange-correlation

energy

.

dx

E„,[n] is,

(3)

Here e„,(n) is given by the Wigner interpolation (in atomic units),

0 458— /r, . —0. 440/(7.

e„,(n) =

The last term in (1) represents

formula

8+r, ) .

(4)

the electrostatic

energy

of the system, where P(x) satisfies Poisson's equation, 2p

dx

=4m[n+(x. ) —n (x)] .

To solve the minimization problem tional (1), write the Euler equation, (A,

4/)[d(d

posed by the func-

'(dn/n dx) ]

nn/dx)/dx+

—,

= '(3m. —,

+ V„,(n)+P(x) —p .

n)

It is convenient to write this equation new independent variable u (x) [n (x)]'

=

(A, /2)d

u

(x)/dx

in terms

(6)

of the

=[ '(3' n) + V„,(n) —,

+P(x) —p]u (x) . Consider now the semi-infinite

n+(x)=noe( —x) .

E [n] = T, [n]+E„,+ —,' P(x)[n (x) —n+(x)]dx

with

f

E„,[n]= n(x)e„,(n)dx

STATEMENT OF THE PROBLEM

Consider the jellium model of a metallic surface. energy functional is

T, [n]=

(LDA),

approximation

metal, then

n+(x)

is

(8)

Here no is the bulk density of the metal. Now study the asymptotic behavior of the solution, both inside and outside the metal. First, discuss the behavior outside the metal. From Eq. (6) it is seen that if one assumes that n (x) = Ae for large x & 0, then (A, /8)co

=P( oo ) —p=@,

(9)

in

where N is the work function and where charge neutrality has been assumed. Note that the exact solution u (x) has a behavior that divers from the behavior of the ThomasFermi solution, which decays only with a power law. Mathematically, this is due to the fact that the gradient

36

1785

(2)

1987

The American Physical Society

BRIEF REPORTS

1786

correction is a singular perturbation term; each new gradient correction term adds higher-order derivatives to the corresponding Euler equation. In the metal interior n (x) must approach np, therefore, we write n (x)=np(1+Q), and linearize Eqs. (6) and (7), obtaining (A. /4)d

=aQ+Q —p,

Q/dx

d 2P dx where the constants

(loa)

TABLE I. Values of the decay constants for several simple metals, as a function of the density parameter r, . Values were ', and Wigner exchange-correlation energy. obtained for A. = —

and p are given by

a= ,'kf+—npd V„,(np)/dn,

(1 la)

p=47rnp .

(1 lb)

(a.u. )

Li

K

3.28 3.99 4.96

Rb Cs

5.23 5.63

dQ

dx

From Eqs. (10a) and (10b) it is seen that, for large x inside the metal, both P(x) — p and Q(x) behave as e",

dx

with k given by (A,

/4)k

—ak +P=O

.

dP dx

(12)

Table I shows the values of the real and imaginary part of k for the alkali metals; it is seen that it is a complex number in all cases; this means that the electronic density n (x) oscillates, n

(x) =np[l+ Ae

"

cos(k;x+5)] .

(13)

These oscillations are similar in structure to the Friedel oscillations found in the self-consistent solution of Lang fact for the and Kohn. This is a largely unknown Thomas —Fermi —von Weizsacker (TFW) function. One must point out, however, that these oscillations are not Friedel osciHations, since their wave number is not 2kf The constants 2 and 5 and their decay is exponential. cannot be determined from the present, linear analysis. It is also interesting to observe that the constant k is also complex even in the absence of exchange and correlation, e„=O, as shown in Table II. This is an unexpected result, since one would expect that the oscillations would be interaction; driven precisely by the exchange-correlation the only possible explanation is that they are driven by the gradient correction. Note also that the exact solution of surface problem satisfies the Buddthe semi-infinite Vannimenus theorem, a fact that could be used in a numerical approach as a test on self-consistency.

II.

de dx

k„ (a. u. )

1.170

1~

0.962 0.774 0.734 0.682

0.924 0.716 0.671 0.611

146

=U

0.661 0.671 0.740 0.767 0.806

(14a)

= (2 /k) [ 1 /2( 3mn) =

k;

(a.u. )

./

+ V„, +]]]]—p]u,

(14b)

(14c)

LU

=4rr[n+(x)

—n (x)] .

(14d)

Consider now the boundary conditions that must be imposed upon the solution. Let us consider the case of a jellium slab of width 2L, with ionic density profile

if x E( L, L), n+(x)= . np

— (15)

0 otherwise .

Observe that the value of the chemical potential p can be chosen as zero; if the integration is started from a point x =R (in the asymptotic region) inwards, then —elf(x —xP )/2 ] /2 (R ) (16a)

v(R)= —p]u (R),

(16b)

P(R) = P( ~ ) —]r[u (R)/p]]

(16c)

w(R)=2iru (R)/p] .

(16d)

Note that p] and ])]( pp ) are related by Eq. (9), with the choice p=0. From the symmetry of the slab one has du (x

=0)

dx

=0,

(17a)

NUMERICAL APPROACH

At first glance it may seem that solving the system under study would hardly pose any difficulty. This, however, is not the case, since the system of equations is not stable. The nature of this instability is mainly electrostatic, since it is only for the correct solution that one satisfies Aside from this very the charge neutrality requirement. important point, it is common knowledge that the system is most easily solved if one uses the dependent variable u (x) previously defined, instead of n (x), since the system becomes somehow less unstable. To solve our system, it is preferable to write it as a systern of first-order differential equations; in this way one can use a Runge-Kutta integration method. The system is

2kf (a.u. )

rs

Metal

Na

(lob)

a

36

TABLE II. Decay parameters of jellium, for e„,(n) =0. The values of the decay constants for Al and Pb are real, therefore the two real solutions are given 2kf Metal

(a.u. )

(a.u. )

Al Pb

2.07 2. 30 2.65 3.28 3.99 4.96 5.23 5.63

1.854 1.669 1.448 1.170

Zn

Li Na

K Rb Cs

0.962 0.774 0.734 0.682

k„ (a.u. )

k; (a.u. )

2.367 2.251 1.810 1.769 1.365 0.959

0.666 0.944 0.361 0.989 0.955 0. 146 0. 175 0.201

0.916 0.859

BRIEF REPORTS

36

1787

TABLE III. Work functions for the alkali metals. Present'

Ref. 4

Ref. 3

Metal

(a.u. )

(eVj

(eV)

(eV)

(eV)

Li

3.28 4.00 4.96 5.23 5.63

3.32 2.60 2. 38 2.33 2.25

2. 87 2. 59 2.29 2.22

3. 11 2.93 2.76 2.71 2.64

3.06 2.74 2.63 2.49

Na

K Rb Cs

Present

3 37 ~

'Jellium model. Pseudojellium model.

dtt(x =0) dx

(17b)

to charge neutrality. Condition (17b) is equivalent To Given co and xo, a solution is uniquely determined. find the proper solution one must satisfy Eqs. (17), which constitute a system of nonlinear equations. Define F(ro, xo) = G co, xp

du (x

=0)

(18)

dx

dP(x

=0)

(19)

dx

To obtain the solution that we seek, we must find the roots of (18) and (19). This is done by Newton's method, which converges rapidly once a reasonable starting point is found. Observe that one must make sure that a true minimum of the functional has been found. NormaHy, it is enough to require that the function u (x) has no nodes.

III. RESULTS The method described above has been applied to study the electronic properties of alkali-metal slabs, in particular, the work function and surface energy as a function of slab width. The results obtained can be described as follows: Concerning the work function it is found that, for the metals studied, it approaches its bulk value very rapidly; for example, a slab of sodium of size 5.0 a.u. already has a work function that corresponds to the semi-infinite surface. The calculated values for the work function are presented in Table III, third column. A comparison with the work functions obtained by Smith and the present work shows that they are quite close, within 0.2 eV, and within 0.5 eV of Lang and Kohn's. For the surface energy the situation is more complex. To describe it properly, the surface energy can be split into its Thomas-Fermi (TF), gradient (gr), electrostatic TABLE IV. Components

components (xc). If one (es), and exchange-correlation looks at the total surface energy as a function of the slab width, it is observed that up to a length of up to 10 a.u. it has not yet converged to its bulk value (it oscillates). The bulk of the contribution to this variation comes from the Thomas-Fermi and the exchange-correlation parts, which are always larger than the gradient and electrostatic parts. The reason of this oscillation can be understood as follows: The density at the center of the slab, n(L), is an oscillatory function of L, and it correlates very well with the (surface) energy oscillations; these oscillations will persist as long as n (L) has not settled to no. This situation reminds one of similar oscillations in the case of small metallic particles. The oscillations in surface energy represent a variation of the order of 10% of the total, so it may be said that the surface energy will remain within these bounds. With this proviso one can take the values given in Table IV as the surface energy of a metal in the TFW approximation. To compare with Warner's results, a calculation was made for a cesium slab of width 5. 1 a.u. The difference between the two solutions is impossible to notice visually, in spite of the fact that the solutions satisfy different boundary conditions. The boundary condition used by Warner was to require the density to vanish at a large (but finite) distance from the metal surface. The present solution, instead, has the correct asymptotic behavior far from the slab. This difference could account for the slight difference between Warner's work function, 8'=2. 24 eV, and the present, 8'=2. 25 eV. Surface energies were not reported in Warner's work; here o. =48 erg/cm, to be compared with Lang and Kohn's o =70 erg/cm . In a recent article, a model has been introduced to calculate the electronic properties of inhomogeneous metallic systems. It was found that this model, the pseudojellium model, is able to describe very accurately the surface energy of simple metals. The procedure here is to modify the

of the surface energy for the alkali metals (jellium model; energies in

erg/cm ). Metal

Li Na

K Rb Cs

—396 —150 —41 —26 —22

&gr

Oes

xc

94 53

45 12

369 187

28 24

3 3 2

68 47 48

20

112 101 59 48 48

Ref. 4

Ref. 3

132

210

111 69

160 100 85

70

BRIEF REPORTS

1788

TABLE V. Surface energies in the pseudojellium Metal

Li Na

K Rb

oTF

—411 —142 —61 —44

107

30

52 25 21

12

~P. Hohenberg and W. Kohn, Phys. Rev. 138, B864 (1964). 2W. Kohn and L. J. Sham, Phys. Rev. 140, A1133 (1965). N. D. Lang and W. Kohn, Phys. Rev. B 1, 4555 (1970); 3, 1215

(1971). 4J. R. Smith, Phys. Rev. 181, 522 (1969}. sC. Warner, in Thermionic Conversion Specialists Conference, San Diego, 1971 (IEEE, New York, 1972). H. F. Budd and J. Vannimenus, Phys. Rev. Lett. 31, 1218

(1973).

model, as calculated with the TFW approach.

ogr

exchange-correlation energy by the addition of an extra term, b, E„,(n), inside of the metal, which amounts to modifying the chemical potential of the jellium to obtain that of the real metal, by adding a correction Ap. With this, the calculated surface energy can be directly compared with experimental data. This was done in Ref. 8 by solving the Kohn-Sham equations, with good results. Here the same procedure is applied, except that the electronic density is directly computed from the solution of the Euler equation (6). The fourth column of Table III shows the results obtained for the work function, again in good order of magnitude agreement with the results of Lang and Kohn. Note, however, that pseudojellium work functions have a tendency to be smaller than their jellium counterparts. This is contrary to what happens when one does a full Lang-Kohn calculation with pseudojellium correction, as it was done in Ref. 8. The reason for this is not clear presently. The surface energy was also studied, with the results shown in Table V. To present the results, the surface energy 0. was split as before, but with an additional Axc component. The behavior as a function of slab size was found to be the same as that the pure jellium case. The surface energies are again in reasonable agreement with experiment. The shape of the solution for the electronic density solun (x) is not very diff'erent from the Thomas-Fermi

36

5

3

&xc

O

420 171 104 80

—3 —13 —11

axc

55

200 90 90 50

tion, since the oscillations that, according to Eq. (13) should be present, are not seen. This could be attributed to the fact that the equations have been solved only for a slab, and not for the semi-infinite surface. However, it seems more likely that the oscillations are of very small amplitude, since they must decay exponentially. In conclusion, the test of the TFW approach that is reported here shows that one can obtain good estimates of the electronic properties of metallic surfaces. The major difficulty here seems to lie in the fact that the equations to be solved are unstable. A solution for this may already have been found. In a recent article, Levy, Perdew, and Sahni proposed an exact equation to treat any system with an exfunctional, such as those plicitly known kinetic-energy proposed by Ma and Sahni. ' It remains to be seen if the instability problem is avoided with that procedure. ACKNOWLEDGMENTS

The author wishes to acknowledge Professor Herbert B. Shore, Professor Viraht Sahni, and Professor John Perdew for their invaluable comments. This work was supported in part by Fondo Nacional de Desarrollo Cientrfico y Tecnologico (FONDECYT) Grant No. 5078 and Departamento de Investigation y Bibliotecas (DIB), Universidad de Chile, Grant No. E-2286-8623.

7W. Ekardt, Phys. Rev. B 29, 1558 (1984); C. A. Utreras-Diaz and H. B. Shore (unpublished). C. A. Utreras-Diaz and H. B. Shore, Phys. Rev. Lett. 53, 2335 (1984); C. A. Utreras-Diaz, Ph. D. dissertation, University of California, San Diego, 1985. M. Levy, J. P. Perdew, and V. Sahni, Phys. Rev. A 30, 2745

(1984). Q. Ma and V. Sahni, Phys. Rev. B 19, 1290 (1979).

~oC.

VOLUME 36, NUMBER 3

15 JULY 1987-II

Metallic surfaces in the Thomas —Fermi —von Wei*sacker approach: Self-consistent solution Constantino

A. Utreras-Diaz

(Received 17 November

1986)

The problem of a metallic surface is studied and solved in the Thomas —Fermi —von Weizsacker approach. The analysis of the asymptotic solutions shows that the electronic density n (x) approaches its bulk value no in the metal interior exponentially, oscillating about it. This behavior is found to be an effect of the von Weizsacker term, rather than of the exchange-correlation interaction, as one may have thought. The Euler equation is solved for a slab geometry, calculating work functions and surface energies of several simple metals. The case of the pseudojellium model, recently introduced, is also considered here. The results are compared with those of the exact Lang-Kohn theory and with those of Smith.

INTRODUCTION

the local-density

The problem of a metallic surface has been studied using a variety of approaches over the years. The progress that we have witnessed in recent years has been made theory' (DFT). largely possible by the density-functional In considering a given problem within the DFT, one can choose to solve the Kohn-Sham equations for the system, an approach that was pioneered by Lang and Kohn for metallic surfaces. The other approach available consists in solving the Euler equation for the electronic density. In the last case one needs to have accurate expressions for the kinetic-energy functional. An alternative method has been to use the variational principle; for the problem of metallic surfaces this was first done by Smith, who minimized the energy with respect to variations of the electronic density within a one-parameter family of functions. The Euler equation was solved by Warner for a cesium slab. However, his discussion of this subject was incomplete, and has remained unnoticed by most workers in the field. This work is organized as follows. In Sec. I the mathematical problem is set up, and some exact results concerning the nature of the asymptotic solutions are discussed. Section II is devoted to the discussion of the numerical approach, boundary conditions, and stability. Numerical results are presented and discussed in Sec. III.

I.

f

The .

(1)

Here n (x) is the electronic density and n+(x) denotes the density of the ionic background. The kinetic-energy functional is taken as the Thomas-Fermi term plus the first gradient correction (the von Weizsacker term),

A,

= '. —,

f

[3(3m. n)

i 10+A(dn/ndx) /8]n

The exchange-correlation

energy

.

dx

E„,[n] is,

(3)

Here e„,(n) is given by the Wigner interpolation (in atomic units),

0 458— /r, . —0. 440/(7.

e„,(n) =

The last term in (1) represents

formula

8+r, ) .

(4)

the electrostatic

energy

of the system, where P(x) satisfies Poisson's equation, 2p

dx

=4m[n+(x. ) —n (x)] .

To solve the minimization problem tional (1), write the Euler equation, (A,

4/)[d(d

posed by the func-

'(dn/n dx) ]

nn/dx)/dx+

—,

= '(3m. —,

+ V„,(n)+P(x) —p .

n)

It is convenient to write this equation new independent variable u (x) [n (x)]'

=

(A, /2)d

u

(x)/dx

in terms

(6)

of the

=[ '(3' n) + V„,(n) —,

+P(x) —p]u (x) . Consider now the semi-infinite

n+(x)=noe( —x) .

E [n] = T, [n]+E„,+ —,' P(x)[n (x) —n+(x)]dx

with

f

E„,[n]= n(x)e„,(n)dx

STATEMENT OF THE PROBLEM

Consider the jellium model of a metallic surface. energy functional is

T, [n]=

(LDA),

approximation

metal, then

n+(x)

is

(8)

Here no is the bulk density of the metal. Now study the asymptotic behavior of the solution, both inside and outside the metal. First, discuss the behavior outside the metal. From Eq. (6) it is seen that if one assumes that n (x) = Ae for large x & 0, then (A, /8)co

=P( oo ) —p=@,

(9)

in

where N is the work function and where charge neutrality has been assumed. Note that the exact solution u (x) has a behavior that divers from the behavior of the ThomasFermi solution, which decays only with a power law. Mathematically, this is due to the fact that the gradient

36

1785

(2)

1987

The American Physical Society

BRIEF REPORTS

1786

correction is a singular perturbation term; each new gradient correction term adds higher-order derivatives to the corresponding Euler equation. In the metal interior n (x) must approach np, therefore, we write n (x)=np(1+Q), and linearize Eqs. (6) and (7), obtaining (A. /4)d

=aQ+Q —p,

Q/dx

d 2P dx where the constants

(loa)

TABLE I. Values of the decay constants for several simple metals, as a function of the density parameter r, . Values were ', and Wigner exchange-correlation energy. obtained for A. = —

and p are given by

a= ,'kf+—npd V„,(np)/dn,

(1 la)

p=47rnp .

(1 lb)

(a.u. )

Li

K

3.28 3.99 4.96

Rb Cs

5.23 5.63

dQ

dx

From Eqs. (10a) and (10b) it is seen that, for large x inside the metal, both P(x) — p and Q(x) behave as e",

dx

with k given by (A,

/4)k

—ak +P=O

.

dP dx

(12)

Table I shows the values of the real and imaginary part of k for the alkali metals; it is seen that it is a complex number in all cases; this means that the electronic density n (x) oscillates, n

(x) =np[l+ Ae

"

cos(k;x+5)] .

(13)

These oscillations are similar in structure to the Friedel oscillations found in the self-consistent solution of Lang fact for the and Kohn. This is a largely unknown Thomas —Fermi —von Weizsacker (TFW) function. One must point out, however, that these oscillations are not Friedel osciHations, since their wave number is not 2kf The constants 2 and 5 and their decay is exponential. cannot be determined from the present, linear analysis. It is also interesting to observe that the constant k is also complex even in the absence of exchange and correlation, e„=O, as shown in Table II. This is an unexpected result, since one would expect that the oscillations would be interaction; driven precisely by the exchange-correlation the only possible explanation is that they are driven by the gradient correction. Note also that the exact solution of surface problem satisfies the Buddthe semi-infinite Vannimenus theorem, a fact that could be used in a numerical approach as a test on self-consistency.

II.

de dx

k„ (a. u. )

1.170

1~

0.962 0.774 0.734 0.682

0.924 0.716 0.671 0.611

146

=U

0.661 0.671 0.740 0.767 0.806

(14a)

= (2 /k) [ 1 /2( 3mn) =

k;

(a.u. )

./

+ V„, +]]]]—p]u,

(14b)

(14c)

LU

=4rr[n+(x)

—n (x)] .

(14d)

Consider now the boundary conditions that must be imposed upon the solution. Let us consider the case of a jellium slab of width 2L, with ionic density profile

if x E( L, L), n+(x)= . np

— (15)

0 otherwise .

Observe that the value of the chemical potential p can be chosen as zero; if the integration is started from a point x =R (in the asymptotic region) inwards, then —elf(x —xP )/2 ] /2 (R ) (16a)

v(R)= —p]u (R),

(16b)

P(R) = P( ~ ) —]r[u (R)/p]]

(16c)

w(R)=2iru (R)/p] .

(16d)

Note that p] and ])]( pp ) are related by Eq. (9), with the choice p=0. From the symmetry of the slab one has du (x

=0)

dx

=0,

(17a)

NUMERICAL APPROACH

At first glance it may seem that solving the system under study would hardly pose any difficulty. This, however, is not the case, since the system of equations is not stable. The nature of this instability is mainly electrostatic, since it is only for the correct solution that one satisfies Aside from this very the charge neutrality requirement. important point, it is common knowledge that the system is most easily solved if one uses the dependent variable u (x) previously defined, instead of n (x), since the system becomes somehow less unstable. To solve our system, it is preferable to write it as a systern of first-order differential equations; in this way one can use a Runge-Kutta integration method. The system is

2kf (a.u. )

rs

Metal

Na

(lob)

a

36

TABLE II. Decay parameters of jellium, for e„,(n) =0. The values of the decay constants for Al and Pb are real, therefore the two real solutions are given 2kf Metal

(a.u. )

(a.u. )

Al Pb

2.07 2. 30 2.65 3.28 3.99 4.96 5.23 5.63

1.854 1.669 1.448 1.170

Zn

Li Na

K Rb Cs

0.962 0.774 0.734 0.682

k„ (a.u. )

k; (a.u. )

2.367 2.251 1.810 1.769 1.365 0.959

0.666 0.944 0.361 0.989 0.955 0. 146 0. 175 0.201

0.916 0.859

BRIEF REPORTS

36

1787

TABLE III. Work functions for the alkali metals. Present'

Ref. 4

Ref. 3

Metal

(a.u. )

(eVj

(eV)

(eV)

(eV)

Li

3.28 4.00 4.96 5.23 5.63

3.32 2.60 2. 38 2.33 2.25

2. 87 2. 59 2.29 2.22

3. 11 2.93 2.76 2.71 2.64

3.06 2.74 2.63 2.49

Na

K Rb Cs

Present

3 37 ~

'Jellium model. Pseudojellium model.

dtt(x =0) dx

(17b)

to charge neutrality. Condition (17b) is equivalent To Given co and xo, a solution is uniquely determined. find the proper solution one must satisfy Eqs. (17), which constitute a system of nonlinear equations. Define F(ro, xo) = G co, xp

du (x

=0)

(18)

dx

dP(x

=0)

(19)

dx

To obtain the solution that we seek, we must find the roots of (18) and (19). This is done by Newton's method, which converges rapidly once a reasonable starting point is found. Observe that one must make sure that a true minimum of the functional has been found. NormaHy, it is enough to require that the function u (x) has no nodes.

III. RESULTS The method described above has been applied to study the electronic properties of alkali-metal slabs, in particular, the work function and surface energy as a function of slab width. The results obtained can be described as follows: Concerning the work function it is found that, for the metals studied, it approaches its bulk value very rapidly; for example, a slab of sodium of size 5.0 a.u. already has a work function that corresponds to the semi-infinite surface. The calculated values for the work function are presented in Table III, third column. A comparison with the work functions obtained by Smith and the present work shows that they are quite close, within 0.2 eV, and within 0.5 eV of Lang and Kohn's. For the surface energy the situation is more complex. To describe it properly, the surface energy can be split into its Thomas-Fermi (TF), gradient (gr), electrostatic TABLE IV. Components

components (xc). If one (es), and exchange-correlation looks at the total surface energy as a function of the slab width, it is observed that up to a length of up to 10 a.u. it has not yet converged to its bulk value (it oscillates). The bulk of the contribution to this variation comes from the Thomas-Fermi and the exchange-correlation parts, which are always larger than the gradient and electrostatic parts. The reason of this oscillation can be understood as follows: The density at the center of the slab, n(L), is an oscillatory function of L, and it correlates very well with the (surface) energy oscillations; these oscillations will persist as long as n (L) has not settled to no. This situation reminds one of similar oscillations in the case of small metallic particles. The oscillations in surface energy represent a variation of the order of 10% of the total, so it may be said that the surface energy will remain within these bounds. With this proviso one can take the values given in Table IV as the surface energy of a metal in the TFW approximation. To compare with Warner's results, a calculation was made for a cesium slab of width 5. 1 a.u. The difference between the two solutions is impossible to notice visually, in spite of the fact that the solutions satisfy different boundary conditions. The boundary condition used by Warner was to require the density to vanish at a large (but finite) distance from the metal surface. The present solution, instead, has the correct asymptotic behavior far from the slab. This difference could account for the slight difference between Warner's work function, 8'=2. 24 eV, and the present, 8'=2. 25 eV. Surface energies were not reported in Warner's work; here o. =48 erg/cm, to be compared with Lang and Kohn's o =70 erg/cm . In a recent article, a model has been introduced to calculate the electronic properties of inhomogeneous metallic systems. It was found that this model, the pseudojellium model, is able to describe very accurately the surface energy of simple metals. The procedure here is to modify the

of the surface energy for the alkali metals (jellium model; energies in

erg/cm ). Metal

Li Na

K Rb Cs

—396 —150 —41 —26 —22

&gr

Oes

xc

94 53

45 12

369 187

28 24

3 3 2

68 47 48

20

112 101 59 48 48

Ref. 4

Ref. 3

132

210

111 69

160 100 85

70

BRIEF REPORTS

1788

TABLE V. Surface energies in the pseudojellium Metal

Li Na

K Rb

oTF

—411 —142 —61 —44

107

30

52 25 21

12

~P. Hohenberg and W. Kohn, Phys. Rev. 138, B864 (1964). 2W. Kohn and L. J. Sham, Phys. Rev. 140, A1133 (1965). N. D. Lang and W. Kohn, Phys. Rev. B 1, 4555 (1970); 3, 1215

(1971). 4J. R. Smith, Phys. Rev. 181, 522 (1969}. sC. Warner, in Thermionic Conversion Specialists Conference, San Diego, 1971 (IEEE, New York, 1972). H. F. Budd and J. Vannimenus, Phys. Rev. Lett. 31, 1218

(1973).

model, as calculated with the TFW approach.

ogr

exchange-correlation energy by the addition of an extra term, b, E„,(n), inside of the metal, which amounts to modifying the chemical potential of the jellium to obtain that of the real metal, by adding a correction Ap. With this, the calculated surface energy can be directly compared with experimental data. This was done in Ref. 8 by solving the Kohn-Sham equations, with good results. Here the same procedure is applied, except that the electronic density is directly computed from the solution of the Euler equation (6). The fourth column of Table III shows the results obtained for the work function, again in good order of magnitude agreement with the results of Lang and Kohn. Note, however, that pseudojellium work functions have a tendency to be smaller than their jellium counterparts. This is contrary to what happens when one does a full Lang-Kohn calculation with pseudojellium correction, as it was done in Ref. 8. The reason for this is not clear presently. The surface energy was also studied, with the results shown in Table V. To present the results, the surface energy 0. was split as before, but with an additional Axc component. The behavior as a function of slab size was found to be the same as that the pure jellium case. The surface energies are again in reasonable agreement with experiment. The shape of the solution for the electronic density solun (x) is not very diff'erent from the Thomas-Fermi

36

5

3

&xc

O

420 171 104 80

—3 —13 —11

axc

55

200 90 90 50

tion, since the oscillations that, according to Eq. (13) should be present, are not seen. This could be attributed to the fact that the equations have been solved only for a slab, and not for the semi-infinite surface. However, it seems more likely that the oscillations are of very small amplitude, since they must decay exponentially. In conclusion, the test of the TFW approach that is reported here shows that one can obtain good estimates of the electronic properties of metallic surfaces. The major difficulty here seems to lie in the fact that the equations to be solved are unstable. A solution for this may already have been found. In a recent article, Levy, Perdew, and Sahni proposed an exact equation to treat any system with an exfunctional, such as those plicitly known kinetic-energy proposed by Ma and Sahni. ' It remains to be seen if the instability problem is avoided with that procedure. ACKNOWLEDGMENTS

The author wishes to acknowledge Professor Herbert B. Shore, Professor Viraht Sahni, and Professor John Perdew for their invaluable comments. This work was supported in part by Fondo Nacional de Desarrollo Cientrfico y Tecnologico (FONDECYT) Grant No. 5078 and Departamento de Investigation y Bibliotecas (DIB), Universidad de Chile, Grant No. E-2286-8623.

7W. Ekardt, Phys. Rev. B 29, 1558 (1984); C. A. Utreras-Diaz and H. B. Shore (unpublished). C. A. Utreras-Diaz and H. B. Shore, Phys. Rev. Lett. 53, 2335 (1984); C. A. Utreras-Diaz, Ph. D. dissertation, University of California, San Diego, 1985. M. Levy, J. P. Perdew, and V. Sahni, Phys. Rev. A 30, 2745

(1984). Q. Ma and V. Sahni, Phys. Rev. B 19, 1290 (1979).

~oC.